Abstract
Understanding the transfer of spin angular momentum is essential in modern magnetism research. A model case is the generation of magnons in magnetic insulators by heating an adjacent metal film. Here, we reveal the initial steps of this spin Seebeck effect with <27 fs time resolution using terahertz spectroscopy on bilayers of ferrimagnetic yttrium iron garnet and platinum. Upon exciting the metal with an infrared laser pulse, a spin Seebeck current j_{s} arises on the same ~100 fs time scale on which the metal electrons thermalize. This observation highlights that efficient spin transfer critically relies on carrier multiplication and is driven by conduction electrons scattering off the metal–insulator interface. Analytical modeling shows that the electrons’ dynamics are almost instantaneously imprinted onto j_{s} because their spins have a correlation time of only ~4 fs and deflect the ferrimagnetic moments without inertia. Applications in material characterization, interface probing, spinnoise spectroscopy and terahertz spin pumping emerge.
Similar content being viewed by others
Introduction
Transfer of spin angular momentum between two subsystems is a common process in modern magnetism research and highly relevant for the implementation of spintronic functionalities^{1}. In contrast to electrical currents, spin transfer can be induced not only by the flow of conduction electrons, but also by torques exerted between the subsystems^{2,3}. A model case of incoherent spin torque is the spin Seebeck effect^{2,3,4,5,6,7} (SSE), which is typically observed at the interface^{3,8,9} of a magnetic insulator (F) and a nonmagnetic metal (N) (see Fig. 1). By applying a temperature difference T^{N} − T^{F}, a spin current with density^{2,10}
across the interface is induced where \({\cal K}\) is the SSE coefficient. Since F is insulating and N nonmagnetic, j_{s} is carried by magnons in F and by conduction electrons in N. It is readily measured in the N layer through the inverse spin Hall effect (ISHE), which converts the longitudinal j_{s} into a detectable transverse charge current j_{c} (Fig. 1). In the case of temperature gradients in the F bulk, magnon accumulation at the FN interface can make an additional contribution to Eq. (1)^{3,11}.
Note that Eq. (1) presumes a static temperature difference and a frequencyindependent SSE coefficient \({\cal K}\). It is still an open question how the SSE current j_{s} evolves for fast temperature variations and in the presence of nonthermal states. Insights into these points are crucial to reveal the role of elementary processes in the formation of the SSE current, for instance magnon creation^{12} in F and spin relaxation^{13} in N. The highfrequency behavior of the SSE is also relevant for applications, such as magnetization control by terahertz (THz) spin currents^{14,15,16} and spintronic THzradiation sources^{17,18,19,20,21}.
In previous timeresolved SSE works, a transient temperature difference T^{N} − T^{F} was induced by heating the N layer with an optical or microwave pulse^{8,9,22,23}. It was shown that Eq. (1) remains valid on the time resolution of these experiments, from microseconds^{8} through to ~0.1 ns (ref. ^{9}) and even down to 1.2 ps (ref.^{23}). To search for the SSE speed limit, even finer time resolution is required, ultimately reaching the 10 fs scale, which resolves the fastest spin dynamics in magnetic materials^{24}.
In this work, we reveal the initial elementary steps of the longitudinal SSE by pushing its measurement to the THz regime. Upon exciting the metal of a prototypical FN bilayer structure with an infrared laser pulse, the dynamics of the spin Seebeck current j_{s} versus time t are determined with a resolution better than 27 fs using the ISHE and electrooptic sampling. We find that j_{s}(t) rises and decays on time scales of ~100 fs. The decay directly follows the cooling dynamics of the N electrons as seen in the transient sample reflectance. An analytical model shows that j_{s}(t) monitors the density of the transient electrons and holes in the metal quasiinstantaneously because their spins have a correlation time of only ~4 fs and deflect the ferrimagnetic moments without inertia. Simulations consistently reveal that the rise of j_{s}(t) mirrors the thermalization process during which the photoexcited electrons approach a Fermi–Dirac distribution. This observation highlights that efficient spin transfer critically relies on carrier multiplication and is driven by conduction electrons scattering off the metal–insulator interface. Our results are relevant for a large variety of optically driven spintransfer processes. Applications in material characterization, interface probing, spinnoise spectroscopy and THz spin pumping come into reach.
Results
Experiment
A schematic of our experimental setup is shown in Fig. 1 and detailed in the Methods section. In brief, we use ultrashort laser pulses (duration 10 fs, center photon energy 1.6 eV, pulse energy 3.2 nJ) from a Ti:sapphire laser oscillator (repetition rate 80 MHz) to excite the metal of yttrium iron garnet (YIG)platinum (Pt) bilayers. Any spin current j_{s}(t) arising in the metal is expected to be converted into a charge current j_{c}(t) by the ISHE with a bandwidth extending into the THz range^{17}.
These extremely high frequencies are, however, inaccessible to electrical measurement schemes. We, therefore, sample the transient electric field of the concomitantly emitted electromagnetic pulse by contactfree electrooptic detection over a bandwidth of 45 THz. This technique allows us to determine the spin current j_{s}(t) with a time resolution better than 27 fs (see Methods and ref.^{25}). To monitor the electron dynamics in the Pt thin film, we also measure its transient reflectance by a timedelayed optical probe pulse (see Fig. 1).
THz emission from YIGPt
Typical THz electrooptic signals S versus time t for a YIG(3 μm)Pt(5.5 nm) bilayer are displayed in Fig. 2a. The signal inverts when the inplane sample magnetization M is reversed. Since the SSE current is expected to be odd in M, we focus on the THzsignal difference S_ = S(+M) − S(−M) in the following.
Figure 2b shows the amplitude of S_(t) as a function of the external magnetic field, along with the sample magnetization M measured by the magnetooptic Faraday effect (see Methods). First, both curves coincide. Second, the THz electric field associated with S_(t) is found to be linearly polarized and oriented perpendicular to M (see Supplementary Fig. 1).
Third, when reversing the layer sequence from FN to NF, S_(t) changes polarity (see Supplementary Fig. 2). Fourth, S_(t) does not depend on the pumppulse polarization (linear and circular, see Supplementary Fig. 3). Finally, as seen in Fig. 2c, the root mean square (RMS) of S_(t) grows approximately linearly with the absorbed pump fluence. These observations are in line with the scenario suggested by Fig. 1.
Impact of the metal layer
To test the relevance of the ISHE, we replace the Pt with a tungsten (W) layer. The resulting S_(t) exhibits a reduced amplitude and reversed sign (Fig. 2d), consistent with previous ISHE works^{26}. On bare YIG and single Pt films, no signal S_(t) is detected above the noise floor (see Supplementary Fig. 4). These measurements provide supporting evidence that the femtosecond pump pulse injects an ultrafast, Mpolarized spin current along the interface normal and into the N layer where the ISHE is operative (see Fig. 1).
Figure 2e shows that even when introducing a 1.9 nm copper (Cu) spacer layer between YIG and Pt, a measurable THz signal persists. Our result is fully consistent with the picture of a heatinduced spin current flowing from cold YIG into hot Pt, traversing the Cu layer. The presence of the Cu film decreases the current amplitude due to loss^{18,27} and the reduced optical excitation density^{18}.
In summary, the THz emission signal S_ exhibits all the characteristics expected for the SSE. We, therefore, regard the THz data of Fig. 2 as a manifestation of the SSE at THz frequencies. Our measurements rule out alternative THz emission scenarios: (i) An anomalous Nernst effect by proximityinduced moments in Pt would be quenched by a Cu spacer layer, in contrast to our data of Fig. 2e. This contribution is, therefore, negligibly small, in agreement with previous results^{28,29}. (ii) Likewise, a photospinvoltaic effect^{30} does not make a noticeable contribution to the THz signal. (iii) A THz signal due to the Nernst effect^{2} in the N layer would be directly proportional to the external magnetic field, in contrast to our observations of Fig. 2b. (iv) Finally, optical orientation of spins by the optical pump beam in YIG^{24} or Pt^{31} would depend on the pump polarization, again in contrast to our observations.
Temperature dependence
As the SSE current depends on the ferrimagnet’s magnetization M (see Fig. 2b), a marked temperature dependence of the THz emission signal is expected. Figure 3a displays the bulk magnetization of the YIG(3 μm)Pt(5.5 nm) sample versus the ambient temperature T_{0} as determined by the Faraday effect. The Faraday signal disappears at the Curie temperature T_{C} = 550 K of bulk YIG. Figure 3b reveals that the RMS of S_(t) and, thus, the THz spin current also decreases with rising T_{0}, but more rapidly than the YIG bulk magnetization. A similar monotonic decrease was seen in static experiments on YIGPt bilayers, where a temperature gradient in the YIG bulk drives the spin current^{32,33}. Fitting the model function \(\left( {T_{\mathrm{C}}  T_0} \right)^\alpha\) to our data yields an exponent of α = 2.0 ± 0.5 (Fig. 3b), close to the exponents 1.5 and 3 found in refs.^{32,33}, respectively. This agreement provides further evidence that the THz signal S_(t) arises from the ultrafast SSE.
Ultrafast spin Seebeck current
Figure 4a displays the THz signal S_(t) from a YIG(3 μm)Pt(5.5 nm) bilayer, measured with a broadband THz electrooptic crystal. It is related to the spincurrent density j_{s}(t) injected into the N layer by a convolution (Eq. (6)) with a transfer function h(t). We determine h(t) by a reference measurement (see Methods). Its shape (inset of Fig. 4a) implies that S_(t) is roughly proportional to the derivative of j_{s}(t).
Knowledge of the transfer function allows us to apply an inversion procedure^{25} to the THz signal waveform (Fig. 4a). We obtain the central experimental result of this study (Fig. 4b): the ultrafast dynamics of the SSE spin current j_{s}(t) induced by an ultrashort laser pulse. The time resolution of the spincurrent transient is better than 27 fs (see Fig. 4b, Supplementary Fig. 5 and Methods section). Note that j_{s}(t) exhibits an ultrafast rise and decay on a time scale of ~100 fs, more than one order of magnitude faster than any SSE response time reported so far^{8,9,22,23}.
Transient reflectance
To identify the mechanisms underlying the ultrafast spincurrent dynamics, we note that they are triggered by optical excitation of the Pt layer. It is, thus, instructive to briefly review the dynamic response of metal thin films to homogeneous ultrafast optical excitation^{34}. Primarily, at t = 0, the absorbed pump energy is deposited in the electronic system, thereby inducing a nonequilibrium electron distribution. Due to electron–electron and electron–phonon scattering, the electrons approach a Fermi–Dirac distribution. Simultaneously, yet with a usually slower time constant \(\tau _{{\mathrm {eph}}}\), the hot electrons cool down by energy transfer to the phonon system.
A few hundreds of femtoseconds after optical excitation, electron and phonon subsystems can often be adequately described by temperatures. Their transient changes ΔT_{e}(t) and ΔT_{ph}(t) are monitored by considering the pumpinduced change ΔR(t) in the sample reflectance, which scales approximately linearly with ΔT_{e}(t) and ΔT_{ph}(t) (ref.^{35}). As seen in Fig. 4c, −ΔR(t) rises rapidly and relaxes toward a constant background. For t > 350 fs, the decay is well described by a monoexponential function with a time constant of \(\tau _{{\mathrm{e  ph}}} = 310\,\pm\, 70\) fs (dashed line in Fig. 4c). We assign this relaxation to energy transfer from the electrons to the phonons. Remarkably, the spin current j_{s}(t) exhibits a very similar decay (Fig. 4b). This observation strongly indicates that j_{s}(t) quasiinstantaneously follows the transient changes ΔT_{e}(t) in the electron temperature on the time scale of electron cooling. It also suggests that the intrinsic response time of the SSE is significantly faster than \(\tau _{{\mathrm{e  ph}}}\).
Dynamic SSE model
To understand this surprisingly fast response and the nature of the initial rise of the spin current (Fig. 4b), we adapt the static SSE theory of ref.^{3} to the dynamic case and employ a linearresponse approach to spin pumping^{36,37}. As detailed in the Methods section, our treatment is based on the microscopic model that is schematically shown in Fig. 5a. In the following, a concise and intuitive summary is given.
According to ab initio calculations^{38}, the spins of the interfacial F and N layers are coupled by an sdexchangelike Hamiltonian^{3,7,39,40} \(J_{{\mathrm{sd}}}{\mathbf{S}}^{\mathrm F} \cdot {\mathbf{S}}^{\mathrm N}\) over a thickness of about one YIG lattice constant a = 1.24 nm. Here, J_{sd} quantifies the coupling strength, and \(\hbar {\mathbf{S}}^{\mathrm F}\) and \(\hbar {\mathbf{S}}^{\mathrm N}\) are the total electron spin angular momenta contained in an interfacial cell of dimension a^{3} on the F and N side, respectively, with ħ denoting the reduced Planck constant. Thermal spin fluctuations s^{F}(t) in F and s^{N}(t) in N cause stochastic effective magnetic fields and, therefore, torques on each other, which cancel in thermal equilibrium.
However, this balance is broken in our experiment by the pump pulse exciting exclusively the Ncell electrons. Consequently, we focus on elementary interactions caused by spin fluctuations in N. After the arrival of the pump pulse, say at time t′, the conductionelectron spins within an N cell give rise to a random field J_{sd}s^{N}(t′) on the Fcell spins^{3} (Fig. 5a). Subsequently, at time t > t′, the Fcell spin has changed dynamically by \({\mathrm{\Delta }}{\mathbf{s}}^{\mathrm F}\left( t \right) = \underline \chi ^{\mathrm{F}}\left( {t  t\prime } \right)J_{{\mathrm{sd}}}{\mathbf{s}}^{\mathrm N}\left( {t\prime } \right)\), where \(\underline \chi ^{\mathrm{F}} = \left( {\chi _{ij}^{\mathrm{F}}} \right)\) is the spin susceptibility matrix of the F cell^{3,36} (Fig. 5b). However, Δs^{F}(t) is canceled by an oppositely oriented field −J_{sd}s^{N}(t′) occurring with equal probability (see Fig. 5c, d). In other words, the averageinduced moment ⟨Δs^{F}(t)⟩ vanishes because ⟨s^{N}⟩ = 0.
Nevertheless, a net effect results from a second interaction of F with J_{sd}s^{N} at time t > t′ (Fig. 5b, d). The corresponding torque J_{sd}s^{N}(t) × Δs^{F}(t) scales with \(J_{{\mathrm{sd}}}^2\) and, therefore, rectifies the random field J_{sd}s^{N}. Its expectation value is parallel to the F magnetization M (Fig. 5b, d). By integration over all firstinteraction times t′ (see Methods section), we find the spin current due to Ncell fluctuations equals
Equation (2) provides the key to understanding the ultrafast dynamics of the SSE. The spincorrelation function \(\langle s_z^{\mathrm{N}}\left( t \right)s_z^{\mathrm{N}}\left( {t\prime } \right)\rangle\) implies that a net spin current only arises if the two interactions with \(J_{{\mathrm{sd}}}{\mathbf{s}}^{\mathrm N}\) occur within the correlation time \(\tau ^{\mathrm{N}}\) of the Ncell spin, that is, for \( {t  t\prime }  \, < \, \tau^{\mathrm{N}}\). The τ^{N} can be estimated by the time it takes an electron to traverse the interaction region of width ~a (Fig. 5a), yielding τ^{N} ~ 4 fs for Pt. As this time constant is shorter than the pumppulse duration, the Ncell spin correlation function mirrors the instantaneous state of the optically excited electrons in the metal.
Interestingly, the Fcell spins react instantaneously, too, because they have no inertia^{41}. This fact is illustrated by the steplike onset of the transverse Fcell susceptibility \(\chi _ \bot ^{\mathrm{F}}\left( t \right) = \chi _{yz}^{\mathrm{F}}\left( t \right)  \chi _{zy}^{\mathrm{F}}\left( t \right)\) at t = 0 (Fig. 5e). Consequently, the spin current follows the dynamics of the electron distribution in the metal without delay.
From fluctuations to generalized temperatures
To put the last conclusion on a more quantitative basis, we note that the fluctuations of the Ncell spin derive from those of the flux of the N electrons incident on the FN interface (see Fig. 5a–d and Methods). We, accordingly, expect that the strength of the current fluctuations scales with the number of available electronic scattering channels, that is, with the number of occupied initial and unoccupied final Bloch states. Indeed, the variance of the current noise is known to be proportional to^{42}
where \(n\left( {{\it{\epsilon }},t} \right)\) is the occupation number of an electron Bloch state at energy \({\it{\epsilon }}\), \(D\left( {\it{\epsilon }} \right)\) denotes the density of Bloch states, k_{B} is the Boltzmann constant, and \({\it{\epsilon }}_{\mathrm{F}}\) is the Fermi energy.
When \(n\left( {{\it{\epsilon }},t} \right)\) is a Fermi–Dirac function at temperature \(T_{\mathrm{e}}^{\mathrm{N}}\left( t \right)\), the term \(n\left( {{\it{\epsilon }},t} \right)\left[ {1  n\left( {{\it{\epsilon }},t} \right)} \right]\) peaks at \({\it{\epsilon }} = {\it{\epsilon }}_{\mathrm{F}}\) with width \(4k_{\mathrm{B}}T_{\mathrm{e}}^{\mathrm{N}}\left( t \right)\) and height 1/4. Therefore, the quantity \(\tilde T_{\mathrm{e}}^{\mathrm{N}}\left( t \right)\) introduced by Eq. (3) becomes equal to \(T_{\mathrm{e}}^{\mathrm{N}}\left( t \right)\), provided \(D\left( {\it{\epsilon }} \right)\) is constant around \({\it{\epsilon }}_{\mathrm{F}}\). The remarkable equality \(\tilde T_{\mathrm{e}}^{\mathrm{N}}\left( t \right) = T_{\mathrm{e}}^{\mathrm{N}}\left( t \right)\) is still satisfied to a good approximation even for the strongly energydependent density of states of Pt at all electronic temperatures relevant to our experiment (see Supplementary Fig. 6). We, consequently, identify \(\tilde T_{\mathrm{e}}^{\mathrm{N}}\left( t \right)\) as a generalized electronic temperature that is applicable to arbitrary nonthermal electron distributions.
Using linearresponse theory (see Methods), we can, thus, express the correlation function \(\langle s_z^{\mathrm{N}}\left( t \right)s_z^{\mathrm{N}}\left( {t\prime } \right)\rangle\) by means of \(\tilde T_{\mathrm{e}}^{\mathrm{N}}\) and the isotropic spin susceptibility χ^{N} of the N cell. As the F layer remains cold at temperature T_{0}, we obtain
where \({\mathrm{\Delta }}\tilde T_{\mathrm{e}}^{\mathrm{N}} = \tilde T_{\mathrm{e}}^{\mathrm{N}}  T_0\) is the pumpinduced increase of the electron temperature of N. Note that Eq. (4) is the desired generalization of Eq. (1) for timedependent temperatures and nonthermal electron distributions of the N layer.
The response function \({\mathrm{\kappa }}^{\mathrm{N}}\left( t \right) \propto J_{{\mathrm{sd}}}^2\chi ^{\mathrm{N}}\left( t \right){\int} {\mathrm{d}} t\prime\chi _ \bot ^{\mathrm{F}}\left( {t  t\prime } \right)\chi ^{\mathrm{N}}\left( {t\prime } \right)\) can be understood as the spin current induced by a δ(t)like change in \(\tilde T_{\mathrm{e}}^{\mathrm{N}}\). It is determined by the susceptibilities of the Fcell and Ncell spins. For N = Pt, we assume an isotropic spin susceptibility^{43,44} χ^{N}(t) that rises steplike and decays with time constant τ^{N} (see Eq. (26) and Fig. 5e). In contrast, \(\chi _ \bot ^{\mathrm{F}}(t)\) is obtained by atomistic spindynamics simulations^{12,45} and exhibits a strongly damped oscillation reflecting the superposition of numerous magnon modes (see Methods and Fig. 5e). The resulting SSE response function \({\mathrm{\kappa }}^{\mathrm{N}}(t)\) is shown in Fig. 5f.
Comparison to measured and simulated electron dynamics
As expected from our qualitative discussion following Eq. (2), κ^{N}(t) (Fig. 5f) has an ultrashort duration on the order of τ^{N}, much faster than the onset of the measured spin current (Fig. 5g). Therefore and because of Eq. (4), the spin current quasiinstantaneously follows the dynamics of the generalized electron temperature of N,
where \({\cal K} = {\int} {\mathrm{d}} t{\mathrm{\kappa }}^{\mathrm{N}}\left( t \right) = {\int} {\mathrm{d}} t{\mathrm{\kappa }}^{\mathrm{F}}\left( t \right)\) is the static SSE coefficient. We now put this conclusion to test by considering the rise and decay dynamics of the measured spin current j_{s}(t) (Fig. 4b).
First, Eq. (5) is fully consistent with the decay of j_{s}(t) for t > 350 fs (Fig. 4b), whose evolution agrees well with the cooling dynamics of the electron bath due to electron–phonon coupling (Fig. 4c). This agreement shows that Eqs. (4) and (5) are valid for thermal electron distributions and on time scales significantly faster than \(\tau _{{\mathrm{e  ph}}} = 310 \pm 70\) fs.
Second, to check Eq. (5) over the phase in which the measured j_{s}(t) rises, we simulate the electron population dynamics \(n\left( {{\it{\epsilon }},t} \right)\) using the Boltzmann equation for excitation conditions close to those in our experiment. Optical excitation, electron–electron and electron–phonon scattering are explicitly taken into account by collision integrals^{46,47} (see Methods). The evolution of the generalized electron temperature \({\mathrm{\Delta }}\tilde T_{\mathrm{e}}^{\mathrm{N}}(t)\) is calculated through Eq. (3) and shown in Fig. 5g. Note that the increase of \({\mathrm{\Delta }}\tilde T_{\mathrm{e}}^{\mathrm{N}}\left( t \right)\) proceeds within ~100 fs, which is much slower than the duration of the pump pulse and the width of the SSE response function κ^{N}(t). The evolution of \({\mathrm{\Delta }}\tilde T_{\mathrm{e}}^{\mathrm{N}}\left( t \right)\) agrees well with that of the measured j_{s}(t) (Fig. 5g), thereby confirming the validity of Eqs. (4) and (5) for time scales much shorter than 100 fs and for nonthermal electron distributions.
To understand the noninstantaneous rise of the generalized electron temperature, we note that \({\mathrm{\Delta }}\tilde T_{\mathrm{e}}^{\mathrm{N}}\left( t \right)\) approximately scales with \({\int _{{\it{\epsilon }} > {\it{\epsilon }}_{\mathrm{F}}} {\mathrm{d}}{\it{\epsilon}}{\mathrm{\Delta }}n\left( {{\it{\epsilon }},t} \right)}\), that is, the pumpinduced number of electrons above the Fermi energy \({\it{\epsilon }}_{\mathrm{F}}\) (Eq. (3)). Initially, photoexcitation induces electrons and holes at approximately half the pump photon energy of \(\hbar \omega _{\mathrm{p}} = 1.6\) eV away from the Fermi energy. However, subsequent scattering cascades lead to thermalization of the electrons, thereby generating roughly \(\hbar \omega _{\mathrm{p}}/k_{\mathrm{B}}T_0 \sim 60\) thermal electron–hole pairs out of each initially photoinduced pair. This carrier multiplication, in turn, strongly increases the generalized temperature and the spin current (Fig. 5g). It can be considered as an experimental confirmation of the notion that the SSE current is due to electrons impinging on the YIGPt interface^{37,38,39,40,41,42,43,44,45,46,47,48,49,50}.
Discussion
The ~100 fs time scale of electron thermalization in Pt as observed here is consistent with timeresolved photoelectron spectroscopy of Pt at roughly comparable excitation densities^{51}. Similarly, for Ru, another transition metal, the number of photoinduced electrons above the Fermi energy^{52} and, thus, \({\mathrm{\Delta }}\tilde T_{\mathrm{e}}^{\mathrm{N}}(t)\) was observed to rise on a time scale of 100 fs for quite similar excitation densities (Fig. 8 in ref. ^{52}). We note that for a more freeelectronlike metal, such as Al, in contrast, electron thermalization is known to proceed significantly faster because of the smaller Coulomb screening parameter^{47}.
While the preceding analysis has focused on the time scales of the SSE current, we now consider the magnitude of the measured and simulated spin current. In our experiment, the SSE efficiency is given by the THz peak field divided by the peak increase of the generalized electron temperature (Fig. 5g) and estimated to be ~2 V m^{−1} K^{−1}. This value is comparable to results from SSE experiments on samples with Pt layers of similar thickness, that is, for static heating (0.1 V m^{−1} K^{−1})^{53} and laser heating at MHz (0.7 V m^{−1} K^{−1})^{8} or GHz frequencies (37 V m^{−1} K^{−1})^{9}. Our modeling also allows us to extract the YIGPt interfacial exchange coupling constant, yielding \(J_{{\mathrm{sd}}} \sim 2\,{\mathrm{meV}}\) or \({\mathrm{Re}}\,g^{ \uparrow \downarrow } \sim 1 \times 10^{18}\,{\mathrm{m}}^{  2}\) in terms of the spinmixing conductance \(g^{ \uparrow \downarrow }\), in good agreement with calculated^{38} and measured values^{54,55}.
We note that the positive sign of the measured spin current j_{s} (Fig. 4b) implies that the magnetization of YIG decreases. The integrated j_{s}(t) is equivalent to increasing the temperature of the thin YIG interfacial layer of thickness a by at most ~50 K (see Fig. 3a). As this value is significantly smaller than the increase of the Pt electron temperature, we can neglect the backaction of the heated YIG layer on the spin current.
Equations (7) and (28) of our analytical theory (see Methods) allow us to discuss the dependence of the THz SSE amplitude on temperature T_{0} (Fig. 3b) in more detail. If we assume that the spincurrent relaxation length in Pt scales linearly with the Pt conductivity, neglect the small variations of the THz impedance Z(ω) versus T_{0} and note that the spin Hall conductivity of Pt is approximately constant over the temperature range considered here^{56,57}, Eq. (7) implies that the T_{0} dependence of the THz SSE signal originates exclusively from the spinSeebeck current j_{s}. Since the Nlayer spin susceptibility is not expected to vary with temperature^{43}, Eq. (28), in turn, shows that the temperature dependence of j_{s} is governed by that of the product \(J_{{\mathrm{sd}}}^2\chi _ \bot ^{\mathrm{F}}\left( {t = 0^ + } \right)\) of the interface exchangecoupling constant and Fcell spin susceptibility. Indeed, previous work^{58,59,60} has provided strong indications that the temperature dependence of the spin susceptibility at interfaces can differ strongly from that of the bulk magnetization and that the interlayer exchangecoupling parameter may be influenced by the temperature of the spacer layer.
So far, our experiments have been restricted to excitation of the metal part of YIGPt. Our modeling, however, allows us to also calculate the SSE response function \({\mathrm{\kappa }}^{\mathrm{F}}\left( t \right)\) related to heating of the F = YIG layer (see Eq. (18)). Note that \({\mathrm{\kappa }}^{\mathrm{F}}\left( t \right)\) exhibits clear features of the susceptibility of the Fcell spins (Fig. 5f). Measurement of \({\mathrm{\kappa }}^{\mathrm{F}}\left( t \right)\) would, therefore, provide insights into magnon dynamics on the unitcell level. If YIG and Pt layers were uniformly and simultaneously heated by a sudden temperature jump, static SSE theory (Eq. (1)) would imply a vanishing current. In contrast, our theory predicts a 100 fs short current burst (Supplementary Fig. 7), which reflects the inherent asymmetry of the FN structure. At times t > 100 fs, the total spin current vanishes, consistent with the familiar static result of Eq. (1).
In conclusion, we measured an ultrafast spin current in the prototypical SSE system YIGPt triggered by femtosecond optical excitation of the metal layer. The current exhibits all the hallmarks expected from the THz SSE. Our dynamic model, based on sdlike exchangecoupled YIGPt layers, can reproduce both the magnitude and the dynamics of the measured ultrafast spin current. It allows us to identify the ultrafast elementary steps leading to the formation of the initial SSE current: optically excited metal electrons impinge on the interface with the magnetic insulator. They apply random torque that is rectified by two subsequent interactions, thereby resulting in a net spin current from YIG into the metal.
The SSE response to heating of the metal layer is quasiinstantaneous for two reasons. First, the total electron spin of a Pt unit cell at the YIGPt interface has a correlation time of less than 4 fs. Second, the YIG spins respond to these fluctuations without inertia. We emphasize that the steplike impulse response of the YIG spins is a feature of all ferromagnetic magnons of YIG and independent of their frequencies, be it megahertz or THz. As a consequence of these instantaneous responses, the SSE current directly monitors the thermalization and cooling of the photoexcited electrons, which both proceed on a subpicosecond time scale.
In terms of applications, the observed ultrafast SSE current can be understood as a first demonstration of incoherent THz spin pumping. Therefore, an instantaneously heated metal layer is a promising transducer for launching ultrashort incoherent THz magnon pulses into magnetic insulators. They may prove useful for magnonbased transport of information, for exerting ultrafast torques on remote magnetic layers^{61} and for spectroscopy of spin waves with nanometer wavelength^{62}. Our results also strongly suggest that coherent spin pumping should be feasible at THz frequencies^{63}.
From a fundamental viewpoint, our experimental approach permits the characterization of the interfacial SSE and the ISHE of metals in standard bilayer thinfilm stacks with a large sample throughput and without extensive microstructuring^{64}. It allows one to alloptically probe the magnetic texture and the exchange coupling at interfaces. Since our setup is driven by a femtosecond laser oscillator rather than a significantly more demanding amplified laser system, our methodology should be accessible to a broad community. As indicated by Eq. (2), the THz SSE current is also sensitive to the local electronspin noise at the highest frequencies, even under conditions far from equilibrium. Such type of spinnoise spectroscopy is difficult to realize with other methods^{42}.
We finally emphasize that the SSE is a model case of incoherent angularmomentum transfer between a spin ensemble and another system^{65}, such as the electronic orbital degrees of freedom, the crystal lattice or a second spin sublattice of a solid. Therefore, our modeling may serve as a blueprint for a large variety of optically driven spin dynamics, for instance ultrafast switching^{66} and quenching^{67} of magnetic order. Our insights highlight the significant role of carrier multiplication in these processes and strongly suggest that lower pump photon energies (ideally on the order of the thermal energy) will substantially shorten the rise time of the angularmomentum transfer and extend its bandwidth to tens of THz.
Methods
Sample preparation
The YIG films (thicknesses of 2, 3 and 5 µm) were grown by liquidphase epitaxy on 500 µm thick gadolinium gallium garnet (GGG) substrates (Innovent e.V., Jena, Germany). The YIG surface was cleaned with isopropyl alcohol and acetone in an ultrasonic bath. In situ argon etching was omitted in order to maintain the integrity of the YIG surface magnetization^{68}.
Subsequently, films of Pt, W, and MgO were grown on YIG using the Singulus Rotaris sputter deposition system. The MgO serves as a protection against oxidation for the W film. Pt and W were grown using DC magnetron sputtering whereas radiofrequency sputtering was used for MgO growth from a composite target. The deposition rates for Pt, W and MgO were 3.1, 1.5 and 0.08 Å s^{−1}, respectively, at a pressure of 5.7 × 10^{−3}, 3.5 × 10^{−3} and 1.8 × 10^{−3} mbar. For the measurements displayed in Fig. 2e, Pt and Cu layers were grown using a homebuilt deposition system with DC magnetron sputtering at rates of 0.7 and 0.63 Å s^{−1}, respectively, at a pressure of 0.01 and 0.025 mbar.
The samples were characterized magnetooptically by the Faraday effect of a beam from a 512 nm laser diode under an angle of incidence of 45°. In this way, hysteresis loops were measured by slowly varying the external magnetic field.
THzemission setup
In the optical experiment, the inplane sample magnetization was saturated by an external magnetic field of 10 mT. For setting the sample temperature T_{0} between 300 and 600 K, a resistive heating coil was attached to the sample holder onto which the sample was glued with a heatconducting silver paste. The temperature was measured with a typeK thermocouple.
As schematically shown in Fig. 1, the sample was excited by linearly or circularly polarized laser pulses (duration 10 fs, center wavelength 800 nm, pulse energy 2.5 nJ) from a Ti:sapphire laser oscillator (repetition rate 80 MHz) under normal incidence from the GGG/YIG side (beam diameter at sample 22 μm fullwidth at halfmaximum of the intensity). The resulting absorbed fluence was 120 µJ cm^{−2}.
The duration of the pump pulse arriving in the Pt layer was optimized by adjusting the optical thickness of a pair of wedged prisms and the number of reflections on a pair of chirped mirrors. As signal, we used the photocurrent generated by the pulse train in a 2photonabsorption photodiode behind a 0.5 mm thick BK7 substrate (groupdelay dispersion of 22 f s^{−2}). In the experiment, the BK7 window was replaced by a 0.5 mm thick GGG substrate^{69} with a groupdelay dispersion of 82 f s^{−2}, yielding an upper bound of 19 fs for the pulse duration.
The THz electric field emitted in transmission direction was detected by electrooptic sampling^{70,71}, where probe pulses (0.6 nJ, 10 fs) from the same laser copropagate with the THz field through an electrooptic crystal. The resulting signal S(t) equals twice the THzfieldinduced probe ellipticity, where t is the delay between the THz and probe pulse. Depending on the signal strength and bandwidth required, we used various electrooptic materials, ZnTe(110) (thickness of 1 mm) and GaP(110) (250 µm). If not mentioned otherwise, all measurements were performed at room temperature in a dry N_{2} atmosphere.
Extraction of the THz current
Generally, the measured electrooptic signal S(t) is related to the THz electric field E(t) directly behind the sample by the convolution
Here, the transfer function h(t) accounts for propagation to the detection unit, as well as the detector response function of the electroopticsampling process. We determined this function by using an appropriate reference emitter^{25}.
The measured transfer function (inset of Fig. 4a) exhibits a sharp bipolar feature around t = 0, which upon convolution with E(t) approximately yields a signal proportional to the derivative of the field, \(S\left( t \right) \propto \partial E(t)/\partial t\). Equation (6) was inverted directly in the time domain by recasting it as a matrix equation. Note that the DC component of h(t) is zero because a DC electric field cannot propagate away from its source. We determined the missing DC component of E(t) by using the causality principle: the pumpinduced charge current inside the sample and, thus, E(t) is zero before arrival of the pump pulse at t = 0.
In the frequency domain, the field E(ω) is related to the spin current injected into the Pt layer by a generalized Ohm’s law^{17}
Here, \(\omega /2\pi\) denotes frequency, and −e is the electron charge. The impedance Z(ω) of the YIGPt bilayer on GGG was determined by THz transmission spectroscopy^{17}. The spin Hall angle of Pt is assumed to be \(\theta _{{\mathrm{SH}}} = 0.1\) (ref.^{72}), and the relaxation length of the ultrafast spin current is \(\lambda _{{\mathrm{rel}}} = 1\) nm (ref.^{17}). Consequently, all transfer functions relating S, E and eventually j_{s} are known, and we can extract j_{s}(t) from the measured THz signal S(t) by inverting Eqs. (6) and (7)^{25}. The polarization of the spin current was calibrated by using a metallic reference emitter^{17}.
Our inversion procedure is illustrated in Fig. 4a, b and Supplementary Fig. 5. For example, the electrooptic signal S_(t) odd in the YIG magnetization (Fig. 4a) approximately scales with the derivative of the field E(t) and, thus, the chargecurrent density \( e\theta _{{\mathrm{SH}\,}}j_{\mathrm{s}}(t)\) (Fig. 4b). We also analyze the THz signal S_{+}(t) even in the YIG magnetization (Supplementary Fig. 5c) and find a charge current that equals a sharp Gaussian peak with a width of 27 fs (Supplementary Fig. 5d). We infer that the time resolution of the spincurrent transient is better than 27 fs. This value is a result of the pumppulse duration in the Pt layer and of the lowpass filtering included in our extraction procedure, which imply a temporal broadening of at most 19 and 24 fs, respectively.
Transient reflectance
To conduct opticalpump reflectanceprobe measurements on a Pt thin film (thickness of 30 nm), the beam of ppolarized laser pulses (duration 14 fs, center wavelength 800 nm) from a cavitydumped Ti:sapphire oscillator (repetition rate 1 MHz) was split into pump and probe pulses at a power ratio of 4. The pump and probe beams were incident onto the sample at angles of 45° and 50°, respectively. The pumpinduced modulation of the reflected probe power was measured using a photodiode and lockin detection and yielded the relative pumpinduced change \({\mathrm{\Delta }}R(t)/R_0\) in the sample reflectance. The pumppulse parameters, the thickness of the Pt film (30 nm), and the absorbed pump fluence (400 µJ cm^{−2}) were chosen such to obtain excitation conditions similar to those used for measuring the spin current (Fig. 4b).
If electrons and phonons of the photoexcited metal film can be adequately described by temperatures and their transient changes ΔT_{e}(t) and ΔT_{ph}(t) are small, the pumpinduced change ΔR(t) in the sample reflectance scales approximately linearly with ΔT_{e}(t) and \({\mathrm{\Delta }}T_{{\mathrm{ph}}}\left( t \right)\) (ref.^{35}). In the absence of transport, energy conservation furthermore implies \({\mathrm{\Delta }}\dot T_{\mathrm e}\left( t \right) \propto {\mathrm{\Delta }}\dot T_{{\mathrm{ph}}}\left( t \right)\), and ΔR(t) becomes proportional to ΔT_{e}(t) plus a constant.
Temperature estimates
The peak electronic temperature induced by the pump pulse is obtained from the simulations of the dynamics of the electron distribution function (see below) and the resulting evolution of the generalized temperature (see Eq. (3) and Fig. 5g). To estimate how strongly the YIG is modified by the ultrafast spin current, we timeintegrate the measured j_{s}(t) (Fig. 4b). The resulting loss of spin angular momentum reduces the magnetization of the first YIG monolayer by 5%, which is equivalent to increasing its temperature by about 50 K (see Fig. 3a). Material parameters relevant for these estimates are summarized in Supplementary Table 1.
Derivation of the SSE current
As illustrated in Fig. 5a–d, interfacial F and N layers of thickness a are coupled by nearestneighbor sdtype exchange interaction. We divide the interfacial plane in N cells of size a^{3} and consider the total electron spin \(\hbar {\mathbf{S}}_\alpha ^{\mathrm{F}}\) and \(\hbar {\mathbf{S}}_\alpha ^{\mathrm{N}}\) contained in an F cell and N cell with index α, respectively. The expectation value of \({\mathbf{S}}_\alpha ^{\mathrm{F}}\) is related to the F magnetization by \(\langle{\mathbf{S}}_\alpha ^{\mathrm{F}}\rangle \propto a^3{\mathbf{M}}\).
According to ab initio simulations^{38}, coupling between F and N spins is given by the sdexchangetype Hamiltonian^{3,7,39,40} \(H_{{\mathrm{sd}}} = J_{{\mathrm{sd}}}\mathop {\sum }\limits_\alpha {\mathbf{S}}_\alpha ^{\mathrm{F}} \cdot {\mathbf{S}}_\alpha ^{\mathrm{N}}\). Therefore, each \({\mathbf{S}}_\alpha ^{\mathrm{N}}\) applies the torque \({\mathbf{S}}_\alpha ^{\mathrm{F}}(t) \times J_{{\mathrm{sd}}}{\mathbf{S}}_\alpha ^{\mathrm{N}}(t)\) on the adjacent \({\mathbf{S}}_\alpha ^{\mathrm{F}}\). Accordingly, the total \(H_{{\mathrm{sd}}}\)related torque exerted by N on F is given by the sum over all cells α. By taking the expectation value, we obtain the average spincurrent density
flowing from F to N, where Na^{2} is the coupled interface area. Note that the tensor of the spincurrent density is given by the tensor product \({\mathbf{j}}_{\mathrm{s}} \otimes {\mathbf{n}} = {\mathbf{j}}_{\mathrm{s}}^{\,\,\,\mathrm{t}}{\mathbf{n}}\) with n being the normal unit vector of the FN interface.
We now split the random observable \({\mathbf{S}}_\alpha ^{\mathrm{F}} = \langle{\mathbf{S}}_\alpha ^{\mathrm{F}}\rangle + {\mathbf{s}}_\alpha ^{\mathrm{F}} + {\mathrm{\Delta }}{\mathbf{s}}_\alpha ^{\mathrm{F}}\) in three contributions: its mean value \(\langle{\mathbf{S}}_\alpha ^{\mathrm{F}}\rangle \propto a^3{\mathbf{M}}\) and its fluctuating part \({\mathbf{s}}_\alpha ^{\mathrm{F}}\), both taken in the absence of interfacial coupling. In contrast, \({\mathrm{\Delta }}{\mathbf{s}}_\alpha ^{\mathrm{F}}\) quantifies the modification due to sdcoupling to the N layer. By applying an analogous splitting to \({\mathbf{S}}_\alpha ^{\mathrm{N}}\), the spin current becomes
It has contributions \({\mathbf{j}}_{\mathrm{s}}^{\mathrm{N}}\) and \({\mathbf{j}}_{\mathrm{s}}^{\mathrm{F}}\) arising from spin fluctuations in N and F, respectively, which cancel in equilibrium. We approximate \({\mathrm{\Delta }}{\mathbf{s}}_\alpha ^{\mathrm{F}}\) to first order in J_{sd}, that is, by the linear response given by the spatiotemporal convolution^{36}
Here, \(\underline \chi ^{\mathrm{F}}\left( {{\mathbf{x}},t} \right) = \left( {\chi _{ii\prime }^{\mathrm{F}}\left( {{\mathbf{x}},t} \right)} \right)\) is the spin susceptibility tensor of the F cell in matrix notation. An analogous expression holds for \({\mathrm{\Delta }}{\mathbf{s}}_\alpha ^{\mathrm{N}}\) with respect to \(\underline {\mathrm{\chi }} ^{\mathrm{N}}\left( {{\mathbf{x}}_\alpha  {\mathbf{x}}_{\alpha \prime },t  t\prime } \right){\mathbf{s}}_{\alpha \prime }^{\mathrm{F}}\left( {t\prime } \right)\). We furthermore assume that spins of different cells have negligible correlation, for instance \(\langle s_{\alpha ,i}^{\mathrm {N}}\left( t \right)s_{\alpha \prime ,i\prime }^{\mathrm {N}}\left( {t\prime } \right) \rangle\propto \delta _{\alpha \alpha \prime }\). By substituting \({\mathrm{\Delta }}{\mathbf{s}}_\alpha ^{\mathrm{N}}\left( {t} \right)\) and \({\mathrm{\Delta }}{\mathbf{s}}_\alpha ^{\mathrm{F}}\left( {t} \right)\) in Eq. (9), we obtain
where \({\mathbf{s}}^{\mathrm {N}} = {\mathbf{s}}_\alpha ^{\mathrm{N}}\) and \({\mathbf{s}}^{\mathrm {F}} = {\mathbf{s}}_\alpha ^{\mathrm{F}}\) are the spins of any conjoined F and N cells, say \(\alpha = \alpha \prime = 1\). The \(\underline {\mathrm{\chi }} ^{\mathrm{F}}\left( t \right) = \underline {\mathrm{\chi }} ^{\mathrm{F}}\left( {{\mathbf{x}}_\alpha  {\mathbf{x}}_\alpha = 0,t} \right)\) and \(\underline {\mathrm{\chi }} ^{\mathrm{N}}\left( t \right) = \underline {\mathrm{\chi }} ^{\mathrm{N}}\left( {{\mathbf{x}}_\alpha  {\mathbf{x}}_\alpha = 0,t} \right)\) can be interpreted as the spin susceptibility of any F and N cell, respectively. Therefore, we have arrived at the picture of a single pair of coupled F–N cells as considered in the main text (Fig. 5a).
In Eq. (11), the difference of the two terms reflects the competition between the torques arising from the fluctuations of the Ncell and Fcell spins. For example, as illustrated by Fig. 5a, b, the first term can be understood as follows: the fluctuating exchange field \(J_{{\mathrm{sd}}}{\mathbf{s}}^{\mathrm {N}}(t)\) due to N exerts torque on the magnetic moment \({\mathrm{\Delta }}{\boldsymbol{s}}^{\mathrm {F}}\left( t \right) = J_{{\mathrm{sd}}}{\int} {\mathrm{d}} t\prime \,\underline {\mathrm{\chi }} ^{\mathrm{F}}\left( {t  t\prime } \right){\mathbf{s}}^{\mathrm {N}}\left( {t\prime } \right)\), which it has induced in F before. As this torque scales quadratically with the noise s^{N}, it does not vanish, provided Δs^{F}(t) results from an earlier time t′ that lies inside the correlation window of the Ncell spin.
The last statement becomes more apparent when we explicitly write out the matrix and vector products in Eq. (11). Consequently, the component \(j_{\mathrm{s}}=j_{{\mathrm{s}}x}\) of the spincurrent density polarized along the sample magnetization M (see Fig. 1) is found to be
where \({\it{\epsilon }}_{xjk}\) denotes the Levi–Civita symbol. The first term of Eq. (12) quantifies the torque due to Ncell spin fluctuations and depends critically on the spin correlation function \(\langle s_j^{\mathrm N}\left( t \right)s_l^{\mathrm N}\left( {t\prime } \right)\rangle\) which typically peaks sharply around time \(t = t\prime\). Any temperature change of the N spins will lead to a (possibly delayed) modification of the spin correlation function and, therefore, a spincurrent response whose time dependence is determined by the spin susceptibility \(\chi _{kl}^{\mathrm{F}}\left( t \right)\) of the ferromagnet F. An analogous interpretation applies to the second term.
Equation (12) couples the dynamics proceeding in F and N. To describe dynamics in the bulk of F and N, Landau–Lifshitz–Bloch or spindiffusiontype equations, respectively, can be used^{3,73}. Note that Eq. (12) is quite generally valid, including the cases of insulating antiferromagnetic F layers and nonthermal states of F and N. If N is isotropic (as is fulfilled for Pt), one has \(\langle s_j^{\mathrm {N}}\left( t \right)s_l^{\mathrm {N}}\left( {t\prime } \right) \rangle\propto \delta _{jl}\langle s_z^{\mathrm {N}}\left( t \right)s_z^{\mathrm {N}}\left( {t\prime } \right)\rangle\), and the first term of Eq. (12) turns into Eq. (2) of the main text. In the following, we first consider thermal states and subsequently extend our treatment to nonthermal electron distributions in the N layer.
From fluctuations to temperatures
To relate the correlation functions in Eq. (12) to temperatures in F and N, we consider the Kubo form of the fluctuationdissipation theorem in the classical limit^{74},
where Θ is the Heaviside step function. The overbar denotes time inversion, that is, \(\bar f\left( t \right) = f\left( {  t} \right)\), and * denotes convolution (see Eq. (6)). Note that strictly this equation refers to equilibrium and cannot be applied to the situation of our experiment where the temperature of N (and F) is generally timedependent.
To derive a fluctuationdissipation theorem for a nonstationary system, we make use of the Langevin theory^{45,74,75,76}, in which the Ncell spin is assumed to be coupled to a bath of timedependent temperature T^{N}(t). In this framework^{74,75}, the spin fluctuations s^{N}(t) arise from a random magnetic field r^{N}(t) the bath applies to the spin system. Assuming r^{N} has no memory and vanishing ensemble average, the intensity of the spin fluctuations is directly proportional to the instantaneous bath temperature,
where the constant A^{N} quantifies how strongly the N bath and the N spins are coupled. By using linear response,
and writing out the convolution (Eq. (6)), we obtain the spin–spin correlation function for a timedependent bath temperature T^{N},
This relationship shows that the temporal structure of the spin susceptibility \(\chi _{ij}^{\mathrm{N}}\) of N determines how quickly the system adapts to a sudden change in T^{N}. In the case of timeindependent T^{N}, Eq. (16) reduces to the familiar Langevinversion of the fluctuationdissipation theorem^{74,75}. Comparison with the Kubotype fluctuationdissipation theorem (Eq. (13)) yields
This constraint on the spin susceptibility function can be used to determine the constant A^{N}. Completely analogous equations are obtained for the Fcell spin.
We now substitute Eq. (16) and its analog for F into Eq. (12) and obtain
with the response functions
and, completely analogously,
Equations (18–20) can be considered as timedependent generalization of the static constitutive relation (Eq. (1)) of the interfacial SSE. It can be shown that in the static limit of timeindependent temperatures, Eq. (18) reduces to Eq. (1), that is, \(j_{\mathrm{s}} = {\cal K} \cdot \left( {T^{\mathrm{F}}  T^{\mathrm{N}}} \right)\), where \({\cal K} = {\int} {\mathrm{d}} t{\mathrm{\kappa }}^{\mathrm{F}}\left( t \right) = {\int} {\mathrm{d}} t{\mathrm{\kappa }}^{\mathrm{N}}\left( t \right).\) The proof makes use of Eqs. (19) and (20), Parseval’s theorem, Eq. (17) and the causality of the spin susceptibilities of F and N.
For an isotropic nonmagnetic metal N with \(\chi _{ij}^{\mathrm{N}}\left( t \right) = \delta _{ij}\chi ^{\mathrm{N}}\left( t \right)\), Eq. (19) implies the somewhat simpler relationship
For the second response function, we obtain
As seen from Eq. (21), the longitudinal spin susceptibility \(\chi _{jj}^{\mathrm{F}}\) of the F cell does not contribute to \({\mathrm{\kappa }}^{\mathrm{N}}\). The reason is that spin fluctuations along different coordinate axes are uncorrelated in the isotropic N layer. For example, the first interaction of the F layer with \(J_{{\mathrm{sd}}}s_j^{\mathrm{N}}\left( {t\prime } \right)\) would induce a change \(\propto \chi _{jj}^{\mathrm{F}}\left( {t  t\prime } \right)J_{{\mathrm{sd}}}s_j^{\mathrm{N}}\left( {t\prime } \right)\) in the Fcell spin, which is parallel to the j axis. Because \(\langle s_j^{\mathrm {N}}\left( t \right)s_l^{\mathrm {N}}\left( {t\prime } \right) \rangle\propto \delta _{jl}\), the only relevant second interaction is due to \(J_{{\mathrm{sd}}}s_j^{\mathrm{N}}\left( t \right)\), again along the j axis. Therefore, no torque results, and the longitudinal \(\chi _{jj}^{\mathrm{F}}\) does not contribute to \({\mathrm{\kappa }}^{\mathrm{N}}\). This cancellation does not occur for \({\mathrm{\kappa }}^{\mathrm{F}}\) because spin fluctuations in F are correlated in different j directions.
Nonthermal electron distributions
Our previous considerations, in particular Eq. (14), presume a thermal bath with temperature T^{N}. To reveal the nature of the bath and to also account for the nonthermal state of the N electrons directly after laser excitation, we extend our model of the N layer. As the fluctuation of the Ncell spin is assumed to arise predominantly from electrons entering and leaving the N cell^{37,48,49,50}, we model the dynamics of the Ncell spin as
Here, \(i_\sigma ^{{\mathrm{in}}}\left( t \right)\) is the current of electrons with spin \(\sigma = \uparrow\) or \(\downarrow\) incident on the cell boundary. Equation (23) implies that a ↑electron arriving at the N cell at time t′ induces a transient variation \(p\left( {t  t\prime } \right)\) of the Ncell spin. Therefore, the function p(t) has a width on the order of \(\tau ^{\mathrm{N}}\), the mean time it takes an electron to traverse the interfacial metal layer. While \(\langle i_\sigma ^{{\mathrm{in}}}\rangle = 0\), the fluctuations of the current can be modeled by the wellknown result^{42}
where \(v_{k,z}\) is the z component of the group velocity of Bloch state k. We assume constant \(v_{k,z}\) and isotropic electronic occupation numbers \(n_k\left( t \right) = n\left( {{\it{\epsilon }}_k,t} \right)\), where \({\it{\epsilon }}_k\) denotes the band structure. Consequently, Eq. (24) simplifies to
where \(\tilde T_{\mathrm{e}}^{\mathrm{N}}\left( t \right)\) is given by Eq. (3) of the main text.
Comparison of Eqs. (23) to (15) and (25) to (14) reveals the remarkable correspondence \(i_ \uparrow ^{{\mathrm{in}}}  i_ \downarrow ^{{\mathrm{in}}} \leftrightarrow {\boldsymbol{r}}^{\mathrm{N}}\), \(p \leftrightarrow \underline \chi ^{\mathrm{N}}\) and \(\tilde T_{\mathrm{e}}^{\mathrm{N}} \leftrightarrow T^{\mathrm{N}}\) between our spinnoise model and Langevin theory. The analogy identifies the orbital degrees of freedom of the N electrons as the bath that is coupled to the Ncell spins. In addition, as discussed in the context of Eq. (3), \(\tilde T_{\mathrm{e}}^{\mathrm{N}}\left( t \right)\) can be interpreted as a generalized electron temperature. We are, therefore, led to set \(T^{\mathrm{N}}\left( t \right) = \tilde T_{\mathrm{e}}^{\mathrm{N}}\left( t \right)\) to good approximation in Eq. (16), thereby extending this fluctuationdissipation relationship of the N layer to nonFermi–Dirac electron distributions.
We note that the definition of a generalized temperature of a nonthermal electron system is not unique and depends on the considered property. The \(\tilde T_{\mathrm{e}}^{\mathrm{N}}\) introduced here quantifies the noise intensity of the stream of conduction electrons incident on the FN interface. It does in general not simply scale with the total excess energy density of the electrons, which was used previously to define a generalized temperature^{47}.
Similar considerations can be applied to the correlation function of the Fcell spin, if one wishes to go beyond the Langevintype result of Eq. (16). According to Eq. (29) and ref.^{11}, the spin current \({\mathbf{j}}_{\mathrm{s}}^{\mathrm{F}}\left( t \right)\) due to Fcell spin fluctuations can be expressed by the occupation numbers of all magnon modes, including nonthermal populations. However, since in our experiment the pumpinduced changes of the YIG layer are negligible, we do not consider this aspect further.
Calculation of \({\mathbf{\kappa }}^{\mathbf{N}}\) and \({\mathbf{\kappa }}^{\mathbf{F}}\)
Our numerical calculations are based on Eqs. (21) and (22). For the N layer, we assume
where \(\tau ^{\mathrm{N}} \sim 4\) and 1 fs, respectively, is determined by using the Fermi velocity of Pt (ref.^{77}) and Cu (ref.^{78}). The Ncell DC spin susceptibility \(\chi _{{\mathrm{DC}}}^{\mathrm{N}}\) is related to the paramagnetic susceptibility^{43} \(\tilde \chi _{{\mathrm{DC}}}^{\mathrm{N}}\) of Pt (ref.^{44}) and Cu (ref.^{79}) through \(\chi _{{\mathrm{DC}}}^{\mathrm{N}} = a^3\tilde \chi _{{\mathrm{DC}}}^{\mathrm{N}}/\mu _0g^2\mu _{\mathrm{B}}^2\), where μ_{0} is the vacuum permeability, g = 2, and μ_{B} is the Bohr magneton. The factor \(a^3\) is required since \(\chi _0^{\mathrm{N}}\) refers to the integrated Ncell volume whereas \(\tilde \chi _0^{\mathrm{N}}\) is given per volume. The factor \(\mu _0g^2\mu _{\mathrm{B}}^2\) accounts for the different units used in the definition of \(\tilde \chi _0^{\mathrm{N}}\) and \(\chi _0^{\mathrm{N}}\).
For F=YIG, we determine the \(\underline {\mathrm{\chi }} ^{\mathrm{F}}\) tensor by the Kubo formula (Eq. (13)) using the equilibrium spin correlation functions \(\langle s_j^{\mathrm F}\left( t \right)s_l^{\mathrm F}\left( {t\prime } \right) \rangle= \langle s_j^{\mathrm F}\left( {t  t\prime } \right)s_l^{\mathrm F}\left( 0 \right)\rangle\) with \(t \,> \, t\prime\) as an input. These functions were calculated by atomistic spindynamics simulations^{12,45,76} in which ~10^{6} Fe^{3+} spins were propagated classically according to the YIG spin Hamiltonian plus a thermal noise field provided by a thermostat with temperature 300 K. Trajectories s^{F}(t) were obtained by summing all 20 Fe^{3+} spins of a selected YIG unit cell. Note that this summation is approximately tantamount to summing up magnon amplitudes over all wavevectors and magnon branches^{12}. The ensemble average was obtained by averaging the product \(s_j^{\mathrm F}\left( {t  t\prime } \right)s_l^{\mathrm F}\left( 0 \right)\) over many trajectories.
Estimate of the SSE coefficient
As a cross check, we use Eq. (21) to estimate the order of magnitude of \({\cal K} = {\int} {\mathrm{d}} t{\mathrm{\kappa }}^{\mathrm{N}}\left( t \right)\). This formula can be simplified using Eq. (17) and yields the spin Seebeck coefficient
where \(\chi _ \bot ^{\mathrm{F}}\left( t \right) = \chi _{yz}^{\mathrm{F}}\left( t \right)  \chi _{zy}^{\mathrm{F}}\left( t \right)\). As \(\chi ^{\mathrm{N}}\left( t \right)\) is localized around t = 0, we approximate \(\left( {{\mathrm{\Theta }} \ast \chi _ \bot ^{\mathrm{F}}} \right)\left( t \right) \approx \chi _ \bot ^{\mathrm{F}}\left( {t = 0^ + } \right)t\), use Eq. (26) and obtain
In the last step, we estimated \(\chi _ \bot ^{\mathrm{F}}\left( {0^ + } \right)\) by solving the equation of motion \(\hbar {\mathrm{\Delta }}{\dot{\mathbf s}}^{\mathrm F} \approx \langle{\mathbf{S}}^{\mathrm F}\rangle \times J_{{\mathrm{sd}}}{\mathbf{s}}^{\mathrm N}\) and comparison to \({\mathrm{\Delta }}{\mathbf{s}}^{\mathrm F} = \underline {\mathrm{\chi }} ^{\mathrm{F}} \ast J_{{\mathrm{sd}}}{\mathbf{s}}^{\mathrm N}\). We find \(\chi _ \bot ^{\mathrm{F}}\left( t \right) = {\mathrm{\Theta }}\left( t \right) \cdot 2\left\langle {{\mathbf{S}}^{\mathrm F}}\rangle \right/\hbar\) for times t ≈ 0, where 〈S^{F}〉 ≈ 7 is the total spin of the YIG unit cell at room temperature. Consideration of Eqs. (5) and (28) and the peak of the measured j_{s}(t) (Fig. 5g) yields the estimate \(J_{{\mathrm{sd}}} \sim 2\,{\mathrm{meV}}\).
Equation (28) also allows us to compare the spin Seebeck coefficient of YIGPt and YIGCuPt. Assuming the J_{sd} is the same for YIGPt and YIGCu interfaces and using Eq. (28), we find that \({\cal K}\) of YIGCu is a factor of about 2 smaller than that of YIGPt because of the different spin susceptibility \(\chi ^{\mathrm{N}}\left( t \right)\) (see above). This difference in \({\cal K}\) provides a further reason for our observation that the YIGCuPt sample delivers a factor of 6 smaller THz emission signal than YIGPt (see Fig. 2e).
Spinmixing conductance
Our equations for the SSE current are formulated in terms of the constant J_{sd} that quantifies the coupling strength of electron spins at the FN interface^{3}. To connect to works^{54,55} that formulate the SSE in terms of the spinmixing conductance \(g^{ \uparrow \downarrow }\), we consider the current \({\mathbf{j}}_{\mathrm{s}}^{\mathrm{F}}\) arising from the fluctuations of the F spins. Assuming an isotropic susceptibility of the Ncell spins and approximating \({\mathbf{s}}^{\mathrm {F}}\left( {t\prime } \right)\) by \({\mathbf{s}}^{\mathrm F}\left( t \right) + {\dot{\mathbf s}}^{\mathrm F}\left( t \right)\left( {t\prime  t} \right)\) in Eq. (11) yields
This relationship agrees with the familiar result for thermal spin pumping, which is usually written as \(\langle{\mathbf{s}}^{\mathrm F}\left( t \right) \times {\dot{\mathbf s}}^{\mathrm F}\left( t \right)\rangle\hbar\,{\mathrm{Re}}\,g^{ \uparrow \downarrow }/4\pi \left\langle {{\mathbf{S}}^{\mathrm F}}\rangle \right^2\) (ref.^{37}). Comparison of the prefactors in both equations and use of Eq. (26) yields
and, thus, \({\mathrm{Re}}\,g^{ \uparrow \downarrow } \sim 1 \times 10^{18}\,{\mathrm{m}}^{  2}\), in good agreement with calculated^{38} and measured values^{54,55}. Material parameters relevant for the calculations and estimates are summarized in Supplementary Table 1.
Electrondynamics simulations
For a realistic simulation of the evolution of the electron distribution function \(n\left( {{\it{\epsilon }},t} \right)\) of a given material, we make use of the Boltzmann equation. Optical excitation, electron–electron and electron–phonon scattering are explicitly modeled by collision integrals^{46,47}. All integrals take the density of states and quantum statistics of electrons and phonons of the material under study into account. For the screened electron–electron and electron–lattice Coulomb interaction, the screening parameter is calculated based on the instantaneous electron distribution function.
Instead of considering the electronic band structure of the material over the complete wavevector space, we introduce an effective oneband model in which an averaged isotropic dispersion relation is derived from the density of states \(D\left( {\it{\epsilon }} \right)\). By tightly discretizing the energy space, we obtain a system of about 2700 coupled integrodifferential equations which was numerically propagated in time. Material parameters relevant for the simulations are summarized in Supplementary Table 2.
Data availability
The data that support the findings of this study are available from the corresponding author upon reasonable request.
References
Sander, D. et al. The 2017 magnetism roadmap. J. Phys. D 50, 363001 (2017).
Bauer, G.E.W., Saitoh, E. & van Wees, B.J. Spin caloritronics. Nat. Mater. 11, 391–399 (2012).
Adachi, H. et al. Theory of the spin Seebeck effect. Rep. Prog. Phys. 76, 036501 (2013).
Chumak, A.V. et al. Magnon spintronics. Nat. Phys. 11, 453–461 (2015).
Chotorlishvili, L. et al. FokkerPlanck approach to the theory of the magnondriven spin Seebeck effect. Phys. Rev. B 88, 144429 (2013).
Boona, S.R., Myers, R.C. & Heremans, J.P. Spin caloritronics. Energy Environ. Sci. 7, 885–910 (2014).
Uchida, K. et al. Spin Seebeck insulator. Nat. Mater. 9, 894–897 (2010).
Agrawal, M. et al. Role of bulkmagnon transport in the temporal evolution of the longitudinal spinSeebeck effect. Phys. Rev. B 89, 224414 (2014).
Schreier, M. et al. Spin Seebeck effect at microwave frequencies. Phys. Rev. B 93, 224430 (2016).
Xiao, J. et al. Theory of magnondriven spin Seebeck effect. Phys. Rev. B 81, 214418 (2010).
Rezende, S.M. et al. Magnon spincurrent theory for the longitudinal spinSeebeck effect. Phys. Rev. B 89, 014416 (2014).
Barker, J. & Bauer, G.E.W. Thermal spin dynamics of yttrium iron garnet. Phys. Rev. Lett. 117, 217201 (2016).
Freeman, R. et al. Evidence for DyakonovPerellike spin relaxation in Pt. Phys. Rev. Lett. 120, 067204 (2018).
Schellekens, A.J. et al. Ultrafast spintransfer torque driven by femtosecond pulsedlaser excitation. Nat. Commun. 5, 4333 (2014).
Razdolski, I. et al. Nanoscale interface confinement of ultrafast spin transfer torque driving nonuniform spin dynamics. Nat. Commun. 8, 15007 (2017).
Olejník, K. et al. Terahertz electrical writing speed in an antiferromagnetic memory. Sci. Adv. 4, 3566 (2018).
Seifert, T. et al. Efficient metallic spintronic emitters of ultrabroadband terahertz radiation. Nat. Photonics 10, 483–488 (2016).
Wu, Y. et al. Highperformance THz emitters based on ferromagnetic/nonmagnetic heterostructures, Adv. Mater. 29, 1603031 (2017).
Yang, D. et al. Powerful and tunable THz emitters based on the Fe/Pt magnetic heterostructure. Adv. Opt. Mater. 4, 1944–1949 (2016).
Seifert, T. et al. Ultrabroadband singlecycle terahertz pulses with peak fields of 300 kV cm^{−1} from a metallic spintronic emitter. Appl. Phys. Lett. 110, 252402 (2017).
Torosyan, G. et al. Optimized spintronic terahertz emitters based on epitaxial grown Fe/Pt layer structures. Sci. Rep. 8, 1311 (2018).
Bartell, J.M. et al. Imaging magnetization structure and dynamics in ultrathin Y_{3}Fe_{5}O_{12}/Pt bilayers with high sensitivity using the timeresolved longitudinal spin Seebeck effect. Phys. Rev. Appl. 7, 044004 (2017).
Kimling, J. et al. Picosecond spin Seebeck effect. Phys. Rev. Lett. 118, 057201 (2017).
Kirilyuk, A., Kimel, A.V. & Rasing, T. Ultrafast optical manipulation of magnetic order. Rev. Mod. Phys. 82, 2731 (2010).
Braun, L. et al. Ultrafast photocurrents at the surface of the threedimensional topological insulator Bi_{2}Se_{3}. Nat. Commun. 7, 13259 (2016).
Sinova, J. et al. Spin Hall effects. Rev. Mod. Phys. 87, 1213 (2015).
Du, C. et al. Enhancement of pure spin currents in spin pumping Y_{3}Fe_{5}O_{12}/Cu/metal trilayers through spin conductance matching. Phys. Rev. Appl. 1, 044004 (2014).
Geprägs, S. et al. Investigation of induced Pt magnetic polarization in Pt/Y_{3}Fe_{5}O_{12} bilayers. Appl. Phys. Lett. 101, 262407 (2012).
Kikkawa, T. et al. Longitudinal spin Seebeck effect free from the proximity Nernst effect. Phys. Rev. Lett. 110, 067207 (2013).
Ellsworth, D. et al. Photospinvoltaic effect. Nat. Phys. 12, 861–866 (2016).
Kruglyak, V.V. et al. Measurement of hot electron momentum relaxation times in metals by femtosecond ellipsometry. Phys. Rev. B 71, 233104 (2005).
Wang, S. et al. Spin Seebeck effect and spin Hall magnetoresistance at high temperatures for a Pt/yttrium iron garnet hybrid structure. Nanoscale 7, 17812–17819 (2015).
Uchida, K. et al. Quantitative temperature dependence of longitudinal spin Seebeck effect at high temperatures. Phys. Rev. X 4, 041023 (2014).
Hohlfeld, J. et al. Electron and lattice dynamics following optical excitation of metals. Chem. Phys. 251, 237–258 (2000).
Hohlfeld, J. et al. Timeresolved thermoreflectivity of thin gold films and its dependence on film thickness. Appl. Phys. B 64, 387–390 (1997).
Šimánek, E. & Heinrich, B. Gilbert damping in magnetic multilayers. Phys. Rev. B 67, 144418 (2003).
Tserkovnyak, Y. et al. Nonlocal magnetization dynamics in ferromagnetic heterostructures. Rev. Mod. Phys. 77, 1375 (2005).
Jia, X. et al. Spin transfer torque on magnetic insulators. Europhys. Lett. 96, 17005 (2011).
Silsbee, R.H., Janossy, A. & Monod, P. Coupling between ferromagnetic and conductionspinresonance modes at a ferromagneticnormalmetal interface. Phys. Rev. B 19, 4382 (1979).
Kajiwara, Y. et al. Transmission of electrical signals by spinwave interconversion in a magnetic insulator. Nature 464, 262 (2010).
Kimel, A.V. et al. Inertiadriven spin switching in antiferromagnets. Nat. Phys. 5, 727 (2009).
Blanter, Y.M. & Büttiker, M. Shot noise in mesoscopic conductors. Phys. Rep. 336, 1–166 (2000).
Nolting, W. & Ramakanth, A. Quantum Theory of Magnetism (SpringerVerlag, Berlin, Heidelberg, 2009).
Fradin, F.Y. et al. Calculation of the electronic structure and related physical properties of platinum. Phys. Rev. B 12, 5570 (1975).
Ellis, M.O.A. et al. The Landau–Lifshitz equation in atomistic models. Low. Temp. Phys. 41, 705–712 (2015).
Rethfeld, B. et al. Ultrafast dynamics of nonequilibrium electrons in metals under femtosecond laser irradiation. Phys. Rev. B 65, 214303 (2002).
Mueller, B.Y. & Rethfeld, B. Relaxation dynamics in laserexcited metals under nonequilibrium conditions. Phys. Rev. B 87, 035139 (2013).
Zutic, I. & Dery, H. Spintronics: taming spin currents. Nat. Mater. 10, 647 (2011).
Berger, L. Emission of spin waves by a magnetic multilayer traversed by a current. Phys. Rev. B 54, 9353 (1996).
Stiles, M.D. & Zangwill, A. Anatomy of spintransfer torque. Phys. Rev. B 66, 014407 (2002).
Lei, C. et al. Hotelectrondriven charge transfer processes on O_{2}/Pt (111) surface probed by ultrafast extremeultraviolet pulses. Phys. Rev. B 66, 245420 (2002).
Lisowski, M. et al. Ultrafast dynamics of electron thermalization, cooling and transport effects in Ru (001). Appl. Phys. A 78, 165–176 (2004).
Kehlberger, A. et al. Length scale of the spin Seebeck effect. Phys. Rev. Lett. 115, 096602 (2015).
Burrowes, C. & Heinrich, B. Spin Pumping at Ytrium Iron Garnet Interfaces. In Magnonics: From Fundamentals to Applications (eds. Demokritov, S.O. & Slavin, A.N.) 129–141 (Springer, Berlin, Heidelberg, 2013).
Weiler, M. et al. Experimental test of the spin mixing interface conductivity concept. Phys. Rev. Lett. 111, 176601 (2013).
Isasa, M. et al. Temperature dependence of spin diffusion length and spin Hall angle in Au and Pt. Phys. Rev. B 91, 019905 (2015).
Vila, L., Kimura, T. & Otani, Y. Evolution of the spin Hall effect in Pt nanowires: size and temperature effects. Phys. Rev. Lett. 99, 226604 (2007).
Lindner, J. et al. T^{3/2} dependence of the interlayer exchange coupling in ferromagnetic multilayers. Phys. Rev. Lett. 88, 167206 (2002).
Almeida, N.S., Mills, D.L. & Teitelman, M. Temperature variation of the interfilm exchange in magnetic multilayers: the influence of spin wave interactions. Phys. Rev. Lett. 75, 733–736 (1995).
Schwieger, S. et al. Spinwave excitations: the main source of the temperature dependence of interlayer exchange coupling in nanostructures. Phys. Rev. Lett. 98, 057205 (2007).
Ralph, D.C. & Stiles, M.D. Spin transfer torques. J. Magn. Magn. Mater. 320, 1190–1216 (2008).
Bossini, D. et al. Macrospin dynamics in antiferromagnets triggered by sub20 femtosecond injection of nanomagnons. Nat. Commun. 7:10645 doi: 10.1038/ncomms10645 (2016).
Bocklage, L. Coherent THz transient spin currents by spin pumping. Phys. Rev. Lett. 118, 257202 (2017).
Cramer, J. et al. Complex Terahertz and direct current inverse spin Hall effect in YIG/Cu_{1–x}Ir_{x} bilayers across a wide concentration range. Nano Lett. 18, 1064–1069 (2018).
Tveten, E.G., Brataas, A. & Tserkovnyak, Y. Electronmagnon scattering in magnetic heterostructures far out of equilibrium. Phys. Rev. B 92, 180412 (2015).
Kirilyuk, A., Kimel, A.V. & Rasing, T. Laserinduced magnetization dynamics and reversal in ferrimagnetic alloys. Rep. Prog. Phys. 76, 026501 (2013).
Koopmans, B. et al. Explaining the paradoxical diversity of ultrafast laserinduced demagnetization. Nat. Mater. 9, 259–265 (2010).
Vélez, S. et al. Competing effects at Pt/YIG interfaces: spin Hall magnetoresistance, magnon excitations, and magnetic frustration. Phys. Rev. B 94, 174405 (2016).
Wood, D.L. & Nassau, K. Optical properties of gadolinium gallium garnet. Appl. Opt. 29, 3704–3707 (1990).
Leitenstorfer, A. et al. Detectors and sources for ultrabroadband electrooptic sampling: experiment and theory. Appl. Phys. Lett. 74, 1516 (1999).
Kampfrath, T., Nötzold, J. & Wolf, M. Sampling of broadband terahertz pulses with thick electrooptic crystals. Appl. Phys. Lett. 90, 231113 (2007).
Obstbaum, M. et al. Inverse spin Hall effect in Ni_{81}Fe_{19}/normalmetal bilayers. Phys. Rev. B 89, 060407 (2014).
Zhu, Y.H., Hillebrands, B. & Schneider, H.C. Signal propagation in timedependent spin transport. Phys. Rev. B 78, 054429 (2008).
Kubo, R. The fluctuationdissipation theorem. Rep. Prog. Phys. 29, 255 (1966).
Balakrishnan, V. Fluctuationdissipation theorems from the generalised Langevin equation. Pramana 12, 301–315 (1979).
Atxitia, U., Hinzke, D. & Nowak, U. Fundamentals and applications of the Landau–Lifshitz–Bloch equation. J. Phys. D 50, 033003 (2017).
Ketterson, J.B. et al. Fermi velocity and Fermi radius in platinum. Solid State Commun. 6, 851–854 (1968).
Ashcroft, N.W. & Mermin, N.D. Solid State Physics (Holt, Rinehart and Winston, New York, 1976).
Moruzzi, V.L., Janak, J.F. & Williams, A.R. Calculated Electronic Properties of Metals (Pergamon Press, New York, 1978).
Acknowledgements
We thank G.E.W. Bauer for stimulating discussions and acknowledge funding by the ERC H2020 CoG project TERAMAG/Grant No. 681917, the collaborative research center SFB TRR 227 Ultrafast spin dynamics (projects B01, B02 and B03), the collaborative research center SFB TRR 173 Spin+X (projects A01, A08 and B02), the Marie Curie FP7 project ITN WALL/Grant No. 608031, the DAAD (SpinNet, MaHoJeRo) as well as the DFG priority programs SPP 1538 SpinCaT and SPP 1666 Topological Insulators.
Author information
Authors and Affiliations
Contributions
T.S.S. and T.K. conceived the experiments. S.J., J.C., S.W.,C.C., G.J. and M.K. fabricated and characterized the samples. T.S.S. carried out the terahertz experiments and optical sample characterization with support from O.G. The transient reflectance measurements were performed by I.R. and A.M. Experimental data were analyzed by T.S.S. and T.K. with contributions from A.M. The theoretical model was developed by T.K. and P.W.B. with contributions from T.S.S. and J.B. Atomistic spindynamics simulations of YIG were conducted by J.B. Electrondynamics simulations of Pt were conducted by S.T.W. and B.R. The manuscript was written by T.K. and T.S.S., with contributions from J.B., I.R., J.C., S.F.M., L.N., A.M., G.J., M.M., S.T.B.G., G.W., B.R., P.W.B., M.W. and M.K. All authors contributed to discussing the results and writing the paper.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing Interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Electronic supplementary material
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Seifert, T.S., Jaiswal, S., Barker, J. et al. Femtosecond formation dynamics of the spin Seebeck effect revealed by terahertz spectroscopy. Nat Commun 9, 2899 (2018). https://doi.org/10.1038/s41467018051352
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s41467018051352
This article is cited by

Ultrahigh spin emission from antiferromagnetic FeRh
Nature Communications (2024)

Magnetoresistive detection of perpendicular switching in a magnetic insulator
Communications Physics (2024)

Timedomain observation of ballistic orbitalangularmomentum currents with giant relaxation length in tungsten
Nature Nanotechnology (2023)

Generation of thirdharmonic spin oscillation from strong spin precession induced by terahertz magnetic near fields
Nature Communications (2023)

Efficient ultrafast fielddriven spin current generation for spintronic terahertz frequency conversion
Nature Communications (2023)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.